Received 6 Jan 2014 | Accepted 25 Apr 2014 | Published 18 Jun 2014 DOI: 10.1038/ncomms4954 Self-assembly of colloid-cholesteric composites provides a possible route to switchable optical materials
K. Stratford1,*, O. Henrich1,*, J.S. Lintuvuori1,*, M.E. Cates1 & D. Marenduzzo1
Colloidal particles dispersed in liquid crystals can form new materials with tunable elastic and electro-optic properties. In a periodic ‘blue phase’ host, particles should template into colloidal crystals with potential uses in photonics, metamaterials and transformational optics. Here we show by computer simulation that colloid/cholesteric mixtures can give rise to regular crystals, glasses, percolating gels, isolated clusters, twisted rings and undulating colloidal ropes. This structure can be tuned via particle concentration, and by varying the surface interactions of the cholesteric host with both the particles and conﬁning walls. Many of these new materials are metastable: two or more structures can arise under identical thermodynamic conditions. The observed structure depends not only on the formulation protocol but also on the history of an applied electric ﬁeld. This new class of soft materials should thus be relevant to design of switchable, multistable devices for optical technologies such as smart glass and e-paper.
1 SUPA, School of Physics and Astronomy, The King’s Buildings, The University of Edinburgh, Edinburgh EH9 3JZ, UK. * These authors contributed equally to this work. Correspondence and requests for materials should be addressed to D.M. (email: [email protected]).
NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications 1 & 2014 Macmillan Publishers Limited. All rights reserved. ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954
hen spherical colloidal particles are mixed into a properties and not to maintain them. (This is the e-paper nematic liquid crystal, they disrupt the orientational paradigm 22 and can lead to huge energy savings.) To explore Worder in the ﬂuid and create defects (disclination lines) such metastability, and switching strategies between states, we in the nematic close to their surfaces. To minimize the free- require multi-unit-cell, time-dependent simulations. These go energy cost, it is generally advantageous for defects to be shared: beyond previous studies of colloidal-BP composites17 but follow therefore, the colloidal particles have a generic tendency to comparable simulations of pure BPs10,21,23, and isolated and aggregate. Such aggregates may further self-assemble into lines1, dimeric colloidal particles in cholesterics24,25. 2D crystals2, planar structures3 or 3D amorphous glasses4. The simulations presented here are representative of a liquid Besides being of fundamental interest to material science, these crystal BP with unit cell size in the range of 100–500 nm (ref. 9) structures may have tunable elastic and optical properties5. Hence and particles with a diameter of around 50 nm. The simulations they offer exciting prospects for applications as biosensors6 or as address both the bulk structure, and the structure that forms new devices7,8. when the colloidal dispersion is conﬁned in a narrow sandwich of However, one may also choose to disperse colloidal particles in width comparable to the unit cell size26. It is seen that a wide a cholesteric, rather than nematic, liquid crystal. The molecules variety of structure is possible and may be inﬂuenced by making up this material are chiral, and this causes their average parameters including the solid volume fraction and the details orientation (described by a director ﬁeld) to rotate in space in a of the anchoring at the colloid surface (and the at the surface of helical manner, rather than remain uniform as in nematics. the conﬁning walls). Further, evidence is found for metastable This typically creates a 1-dimensional periodic structure, called switching of this structure in an applied electric ﬁeld. Details of the cholesteric phase, whose wavelength is the pitch, p. The the computational approach are set out in the Methods section, periodicity can, however, become fully three-dimensional (3D) while simulation parameters are reported in the Supplementary in the so-called blue phases (BPs)9. BPs arise because the Methods. director ﬁeld can twist around more than one direction at once (see the cartoon in Supplementary Fig. 1). Such double twist regions (generally cylinders) are energetically favoured at high Results enough molecular chirality, but lead to geometric frustration Structure in bulk BPI. We show in Fig. 1a–d the ﬁnal state because it is impossible to tile the whole 3D space with structures of four simulations in which we ﬁrst equilibrated a double twist cylinders without also introducing ‘disclination stable BPI disclination network in bulk (with periodic boundary lines’. (These are singular topological defects on which the conditions) and then dispersed colloidal particles at random director ﬁeld is undeﬁned.) In BPs, these disclination lines within it. Among dimensionless control parameters are the par- themselves either form a 3D periodic regular lattice (in so ticle solid volume fraction f (f ¼ 1% or 5%); the ratio r¼R=l of called BPI and BPII) or remain disordered (BPIII)10. BPs are particle radius to the BP lattice parameter l (here r ’ 0:14) and stabilised by the tendency of chiral molecules to twist, but the ratio w ¼ WR/K where W is the anchoring strength of the destabilised by the cost of forming topological defects (which cholesteric at the particle surface and K is the elastic constant of locally diminish the molecular alignment). In conventional the liquid crystal. The anchoring strength is deﬁned such that cholesteric materials9, this balance is only achievable in a W40 imparts a preferred orientation to the director ﬁeld at the narrow temperature range of a few degrees, around the onset of particle surface. This orientation can be either normal to the liquid crystalline ordering. However, recent advances in surface or in a plane tangential to the surface, a property related formulation have widened this stability range enormously11–14. to surface chemistry in experimental systems. We choose Most recently, templated BPs with a stability range of À 125 to w ¼ 0.23, 2.3 that are within typical experimental range4. This 125 °C have been reported15, paving the way to applications of parameter can be viewed as the ratio of the anchoring energy, BPs in operational display devices. WR2, to the elastic energy scale for distortion KR. Besides being remarkable materials in themselves, BPs offer For a single colloidal particle in a nematic ﬂuid, w controls the signiﬁcant promise as hosts for dispersing colloidal particles. formation of a local topological defect at the particle surface5, Because BPs contain a disclination network even in the absence of with weak distortion of the nearby ﬂuid at small w. In the particles, they can potentially template colloidal self-assembly. colloidal-BP system, w also plays a determining role in the ﬁnal This was proved recently by simulations of BP-dispersed composite structure. When w is small (Fig. 1a,b; Supplementary nanoparticles that exclude the surrounding liquid crystal Movies 1 and 2), the attraction of particles to the disclination but otherwise have negligible surface interaction with it (to give lattice causes the lattice to become covered by particles, with little a so-called ‘weak anchoring’ regime)16,17. Such particles are disruption of its long-range order. Thus, a templated colloidal attracted to the disclination network in BPs: by covering up the crystal is created, as ﬁrst reported in ref. 17. Interestingly, the defect cores, the high elastic energy cost of those regions is weak but ﬁnite anchoring apparently creates an elastic force avoided. The pre-existing order of the defect network then between the colloidal particles, which leads to very slow dynamics templates particles into a regular colloidal crystal of the same (Supplementary Fig. 4) and the formation of small colloidal lines periodicity. Because this structure has a wavelength in the visible within disclinations, especially for dilute samples (Fig. 1a). It range, the resulting material should inherit (and probably seems likely that polymer-stabilized BPs11 work by a similar enhance) the incomplete photonic bandgap of the parent BP, as principle to this small w case, with a weak segregation of exploited for instance in laser devices12; for related possibilities monomers towards the defect regions. see ref. 18. For large w (Fig. 1c,d; Supplementary Movies 3 and 4), the A second compelling reason to study colloidal-BP composites picture changes markedly. Each colloidal particle now disrupts is that, even without particles, BPs can show several competing signiﬁcantly the order of the nearby ﬂuid, with defect formation metastable free-energy minima, corresponding to different close to its surface5. The resulting strong disruption of local liquid topologies of the defect network19,20, with a strong dependence crystalline order around each particle leads now to a strong on applied electric or magnetic ﬁelds21. Adding particles is likely interparticle attraction. This restructures the disclination network to further enrich the free-energy landscape, creating composites completely, destroying the long range order of the original BPI that might be promising candidates for bistable or multistable topology. Most notably, particle aggregation favours the devices, in which energy is needed only to switch optical formation of defect junctions, where four disclinations meet.
2 NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications & 2014 Macmillan Publishers Limited. All rights reserved. NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954 ARTICLE
Figure 1 | Bulk blue phase structures. Snapshots of the states obtained after dispersing a suspension of colloidal nanoparticles within a cholesteric liquid crystal in the BPI-forming region. a–d correspond to the case of a dispersion of particles in a pre-equilibrated BPI phase; e–h are obtained by dispersing colloids in an isotropic phase and then quenching into the range where BPI is stable, leading to the formation of an amorphous, BPIII-like, disclination network. Structures correspond to (a) and (e) w ¼ 0.23 and f ¼ 1%; (b) and (f) w ¼ 0.23 and f ¼ 5%; (c) and (g) w ¼ 2.3 and f ¼ 1%; (d) and (h) w ¼ 2.3 and f ¼ 5%. The anchoring of the director ﬁeld to the colloidal surface is normal. (For the full parameter list used to generate Figs 1–3 see Supplementary Notes.) For clarity, only a portion of the simulation box is shown its linear extent being ’ 28R (one-eighth of the total volume); the full structures are shown in Supplementary Figs 2 and 3.
This structural motif is present in the unit cell of BPII rather than interparticle forces again dictate the self-assembly. At low BPI (and also seen in the amorphous BPIII (ref. 10)). The particle concentrations, discrete particle clusters decorate an amorphous clusters are disjoint at low volume fractions (f ’ 1 % ), but they defect lattice (Fig. 1g), whereas at higher f a percolating network interact elastically via the connecting disclinations. At larger f, of colloidal strands (the gel in Fig. 1h) is again seen. The the aggregates join up to form a percolating colloidal cluster, structures in Fig. 1a–h have been followed for B20 ms (see which essentially templates the disclinations rather than Supplementary Fig. 4); they correspond to either very slowly vice versa. evolving states or deep metastable minima (elastic interactions are As colloidal-nematic composites4, all the structures in of order KR and dwarf thermal motion, see Supplementary Fig. 4 Fig. 1a–d should be soft solids, of nonzero elastic modulus G at and refs 5,18). low frequency. This contrasts with pure BPs, where G ¼ 0 as the It may be possible to anneal the structures obtained via the ﬂuid can ﬂow with a ﬁnite viscosity via permeation of molecules quench route, although we have not attempted this in simulation. through a ﬁxed defect lattice27,28. We expect the structures in The results presented suggest that even when starting with Fig. 1a–c to be only weak gels, as here the defect network colloidal particles randomly dispersed in an ordered BP, the percolates but particle contacts do not. This is broadly similar to particles are able to distort the structure (Fig. 1a,b). This suggests the cholesteric-nanoparticle gel reported in ref. 29 (with Go1 that it would be difﬁcult to identify a quench protocol which Pa). In contrast, the colloidal gel structure in Fig. 1d should be would lead to less, rather than more, disorder. much more resistant mechanically, due to the formation of a thick percolating particle network. The structure is now akin to that of the self-quenched glass found in colloidal-nematic Structures in conﬁned BPI. In display devices and other optical composites4 at much higher volume fraction (over 20% as applications, it is typical for liquid crystals to be strongly conﬁned opposed to below 5% here), for which GB103 Pa. This ﬁgure is (and subject to strong boundary effects), in contrast to the bulk consistent with an estimate obtained by comparing the geometries considered above. We therefore next describe how mechanical properties of the network of defects stabilized by colloidal suspensions self-assemble in thin sandwiches (thickness colloidal particles with those of rubber30 for the relevant h¼ 1:75 l), whose conﬁning walls can favour either tangential simulation parameters (see Supplementary Table 1). (planar degenerate) or normal (homeotropic) orientation of the A more practical protocol for including particles in a BPI director ﬁeld. For simplicity, we here impose one or the other as a phase is to disperse the particles at random in an isotropic strict boundary condition. phase and then quenching this into the temperature range where Figure 2a–d shows the case of normal wall anchoring on BPI is stable. Here we know that, without particles, the kinetics varying f and w. We quench from the isotropic to the ordered can favour disordered (BPIII-like) intermediates, which may be phase as was done in Fig. 1e–h, and again ﬁnd a metastable, long lived or even metastable23. Figure 1e–h shows outcomes of amorphous disclination network (see Supplementary Methods). such a quench protocol with the same parameter sets as in The resulting colloidal-cholesteric composites are somewhat Fig. 1a–d. For small w, the particles again decorate the similar to those seen in the bulk: for small w the particles are disclination lines, but are this time templated onto an templated by the network (Fig. 2a,b), whereas for large w we amorphous network rather than an ordered one. Increasing the observe isolated clusters (Fig. 2c) and percolated colloidal gels volume fraction (Fig. 1f) leads to a more even coverage with a (Fig. 2d), for f ¼ 1 and 4%, respectively. There are, however, better deﬁned particle spacing. In contrast, for large w, strong signiﬁcant effects of the conﬁning walls. First, the normal
NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications 3 & 2014 Macmillan Publishers Limited. All rights reserved. ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954
Figure 2 | Conﬁned blue phase structures. Snapshots of the steady states obtained when a dispersion of colloids in the isotropic phase is placed in a sandwich geometry and then quenched into a regime where BPI is stable in the bulk. Both top and side views are provided. The anchoring of the director ﬁeld at the walls is normal for a–d and planar for e–h. Structures correspond to (a) and (e) w ¼ 0.23 and f ¼ 1%; (b) and (f) w ¼ 0.23 and f ¼ 4%; (c) and (g) w ¼ 2.3 and f ¼ 1%; (d) and (h) w ¼ 2.3 and f ¼ 4%. As in Fig. 1, only one quarter of the simulation box is shown for clarity (its horizontal extent being ’ 56R and vertical extent ’ 24R in the narrow direction); the full structures are shown in Supplementary Figs 5 and 6. anchoring at the wall recruits particles there, giving (for the show that the individual structural motifs are actually rather chosen h) a density enhancement of the colloid particles at both similar: templated lines for weak anchoring and clusters for walls (see side-views in Fig. 2a–d). Second, the clusters formed at strong anchoring. large w are themselves anisotropic with an oblate habit. These clusters are similar to those reported experimentally for large colloid particles in a cholesteric (but non-BP) host31. Switching in electric ﬁeld. An interesting question, relevant for Figure 2e–h shows comparable simulations for planar wall applications to devices, is whether these structures can be mod- anchoring. Without colloidal particles, planar anchoring results in iﬁed, or switched, with electric ﬁelds. Figure 3 addresses this a regular cholesteric helix, with axis perpendicular to the question, starting from amorphous BP III, this time at a higher boundary walls. This twisted texture develops via a set of defect chirality. Dispersing colloidal particles in this network results in loops, which shrink and disappear to leave a defect-free sample. the particle occupying the available nodes, where the order However, dispersing particles with small w arrests the loop parameter is low (Fig. 3a; Supplementary Movie 5). Applying a shrinking process, stabilizing twisted rings (Fig. 2e) at small f, high enough ﬁeld along the x direction leads to a switching to a and more complicated double-stranded structures at larger f new phase, where colloidal arrays ﬁt within a network with dis- (Fig. 2f). For larger w, we observe thick colloidal ‘ropes’ about ﬁve torted hexagonal cells (Fig. 3b and Supplementary Fig. 7; particles across (Fig. 2g,h). These ropes undulate to follow the Supplementary Movie 6). Remarkably, on ﬁeld removal this chiral structure of the underlying ﬂuid. On increasing the density, honeycomb structure does not ﬁnd its way back to the conﬁg- they develop branch points and ﬁnally again approach a uration before switching on the ﬁeld, but gets stuck into a meta- percolating gel morphology. Note that planar wall anchoring is stable structure (Supplementary Fig. 7), with residual anisotropy incompatible with the normal anchoring on the colloidal particles along the ﬁeld switching direction. Cycling the ﬁeld along the x (for w 40), which are thus repelled from both walls (see the side and y directions leads to distinct metastable structures, which are views in Fig. 2e–h). retained after ﬁeld removal (Supplementary Figs 8 and 9). The degree of similarity between the bulk and conﬁned We note that for the ﬂuid parameters used here, the ﬁeld-induced structures is somewhat masked by the local change in particle changes are irreversible with the weakly anchoring colloid density in the conﬁned case. If one allows for this, Figs 1 and 2 particles. The mesophase without colloid particles undergoes a
4 NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications & 2014 Macmillan Publishers Limited. All rights reserved. NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954 ARTICLE
S (k) 100
0.1 k z
S (k) 400 100
0.1 k z
Figure 3 | Structure in electric ﬁeld. Steady states obtained when a dispersion of colloids is inserted into a thermodynamically stable bulk BPIII with and without applied external electric ﬁeld. Panel a shows the situation in zero ﬁeld, and panel c the situation when the applied ﬁeld is in the x-direction (perpendicular to the plane of the paper). Panels b and d show one plane of the three-dimensional structure factor S(k) computed from the positions of the particles, with wavevector kx ¼ 0, corresponding to a and c, respectively. With ﬁeld, the disclinations form a honeycomb pattern with hexagonal ordering perpendicular to the ﬁeld direction; this is reﬂected in the structure factor. Simulations use weakly anchoring particles w ¼ 0.23 and a volume fraction of f ¼ 5% (see Supplementary Notes for full list of parameters). The full simulation with a box size of ’ 56R is shown. reversible ordering transition10; the reversibility is retained in the concentration and the anchoring conditions at sample walls. presence of particles only if their anchoring is very weak. We have also shown that electric ﬁelds can be used to switch between metastable states, providing a possible route to future multistable device applications. Discussion How do these simulations relate to experiment? Several authors The surprising wealth of colloidal-BP composites obtained in have used nanoparticles in the context of stabilizing BPs32,33. Figs 1–3 is the complex consequence of a simple competition These nanoparticles are typically a few nanometres in size, in between two self-assembly principles. First, BPs provide a three- which case stabilization is explained by the mechanism of defect dimensional template onto which colloidal particles are attracted removal. Experiments suggest this mechanism is also relevant for so as to reduce the elastic stresses arising at the disclination larger particles in the range of 40–70 nm (ref. 34), which is cores17. Second, colloidal intrusions in a liquid crystal raise the consistent with the current simulations. However, the mechanism free energy locally; sharing this cost creates a generic tendency to is observed to be less efﬁcient for particles above 100 nm, where aggregate into clusters4. Which of these factors dominates particles may start to disrupt longer-range liquid crystal order34. depends on w, a dimensionless measure of the anchoring While the ﬁeld of self-assembly with nanoparticles is relatively strength of the director ﬁeld at the colloidal surface. For w1, new35, nanoparticles have also been used in both nematic36 and the templating principle dominates. Colloidal crystals, gels or chiral liquid crystals37 as host ﬂuid templates. The variation of twisted rings can then arise. For w1, interparticle attractions structure seen in our simulations suggest that some careful defeat the templating tendency, and we predict disconnected characterization of parameters such as surface anchoring of aggregates, percolating gels or helical colloidal ropes. In both particles (which are often stabilised, or even functionalised with cases, control is offered by the process route, colloidal surface ligands), together with those associated with any
NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications 5 & 2014 Macmillan Publishers Limited. All rights reserved. ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954
conﬁning surfaces or interfaces, is required to understand the Surface free energy. In addition to the ﬂuid free energy density f(Qab), a surface ﬁnal structure and to be able to reproduce it with a given free energy density is also present to represent the energetic cost of anchoring at a experimental protocol. The identiﬁcation of a model system that solid surface. In the case of normal anchoring, the surface free-energy density (per unit area) is could allow unambiguous comparison between experimental systems and simulation would be extremely useful. Such a system 0 1 0 2 fsðQab; QabÞ¼ WðQab À QabÞ ; ð7Þ might adopt particles of diameter in the range 50 nm or above, 2 0 which allows a coarse-grained simulation approach of the type where Qab is the preferred order parameter tensor at the solid surface, and W is a used here to be adopted, which can then capture the large-scale constant determining the strength of the anchoring. In the case of planar anchoring, a slightly more complicated expression is required to allow for structure required to compare with experiment. In the same vein, 0 degeneracy (see, for example, ref. 41). The determination of Qab for normal and detailed surface chemistry is difﬁcult to represent in coarse- planar anchoring is discussed below. For a colloidal particle of radius R,the grained simulations, so heavily functionalized particles might be strength of the surface anchoring compared with the bulk ﬂuid elastic constant may avoided. be quantiﬁed by the dimensionless parameter WR/K. For small values of this 38 parameter, the presence of a particle surface should have little impact on the local We have not explored in this work switchability by ﬂow , ﬂuid LC ordering. but this could again be inherited from the underlying BP dynamics19,28, in which case the same materials may also be 39 Dynamics of the order parameter. A framework for the dynamics of liquid relevant to the emerging technology of optoﬂuidics . crystals is provided by the Beris-Edwards model42, in which the time evolution of the tensor order parameter obeys Methods ðÞ@t þ un@n Qab À Sab¼ GHab: ð8Þ Thermodynamics. The thermodynamics of the cholesteric liquid crystal can be described by means of a Landau-de Gennes free energy functional F, whose In the absence of ﬂow, equation (8) describes a relaxation towards equilibrium on a density is written as f: timescale determined by a collective rotational diffusion constant G. This relaxation Z is driven by the molecular ﬁeld Hab, which is the functional derivative of the free F½Q¼ d3rf ðÞQðrÞ : ð1Þ energy with respect to the order parameter42: dF 1 dF This free-energy density f ¼ f(Q) may be expanded in powers of the order para- Hab¼À þ dabTr : ð9Þ meter Q and its gradients; Q is a traceless and symmetric tensor, which is denoted dQab 3 dQab from now on in subscript notation as Qab. The largest eigenvalue q and corre- The tensor Sab in equation (8) completes the material derivative for rod-like 42 sponding eigenvector na of Qab describe the local strength and major orientation molecules . It couples the order parameter to the symmetric and antisymmetric axis of molecular order. The theory based on the tensor Qab, rather than a theory parts of the velocity gradient tensor Wab qbua. The symmetric part Aab and the based solely on the director ﬁeld na(r), allows treatment of disclinations (defect antisymmetric part Oab are deﬁned as lines) in whose cores na is undeﬁned. 1 ÀÁ Explicitly, the-free energy density is: A ¼ W þ W ; ð10Þ ab 2 ab ba 1 1 2 1 1 2 2 f ðQabÞ¼ A0 1 À g Q À A0gQabQbgQga þ A0gðQ Þ and 2 3 ab 3 4 ab ð2Þ ÀÁ 1 2 1 2 1 þ Kðe @ Q þ 2q Q Þ þ Kð@ Q Þ : Oab¼ Wab À Wba : ð11Þ 2 agd g db 0 ab 2 b ab 2 2 Here, repeated indices are summed over, while terms of the form Qab should be This full coupling term is then expanded to read QabQab; eagd is the permutation tensor. The ﬁrst three terms are bulk free-energy density whose overall scale is set by A (discussed further below); g 1 0 Sab¼ðÞxAan þ Oan Qnb þ dnb is a control parameter related to a reduced temperature. Varying the latter in the 3 absence of chiral terms (q0 ¼ 0) gives an isotropic-nematic transition at g¼ 2:7 with 1 ÀÁ g þ Qan þ dan xAnb À Onb ð12Þ a mean-ﬁeld spinodal instability at ¼3. 3 The remaining two terms of the free-energy density in equation (2) describe 1 distortions of the order parameter ﬁeld. In theoretical work and when describing a À 2x Qab þ dab QnnWnn: generic rather than a speciﬁc system, it is conventional9,40 to assume that splay, 3 bend and twist deformations of the director are equally costly, that is, there is a Here, x is a material dependent that controls the relative importance of rotational single elastic constant K. The parameter q is related to the helical pitch length p via 0 and elongational ﬂow for molecular alignment, and determines in practice how q ¼ 2p/p, describing one full turn of the director in the cholesteric phase. 0 the orientational order responds to a local shear ﬂow. In all cases, the value used There are two dimensionless numbers, which are commonly referred to as k, here is x ¼ 0.7, which is within the ‘ﬂow aligning’ regime, where molecules align the chirality, and t, the reduced temperature9, which can be used to characterize at a ﬁxed angle (the Leslie angle) to the ﬂow direction in weak simple shear40. The the system. In terms of the parameters in the free-energy density, these are: value of the collective rotational diffusion used in all simulations is G ¼ 0.5 in 27ð1 À g=3Þ simulation units. t¼ ð3Þ g sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Hydrodynamics. The momentum evolution obeys a Navier-Stokes equation 108 Kq2 driven by the divergence of a generalized stress Pab: k¼ 0: ð4Þ g A0 r@t ua þ rub@bua¼@bPab: ð13Þ
If the free-energy density (equation (2)) is made dimensionless, t appears as The pressure tensor Pab is, in general, asymmetric and includes both viscous and prefactor of the term quadratic in Qab, whereas k quantiﬁes the ratio between bulk thermodynamic components: and gradient free-energy terms. The chirality and reduced temperature may be used to characterize an equilibrium phase diagram of the BPs in bulk cholesteric Pab ¼Àp0dab þ Zf@aub þ @buag 9,21 liquid crystals . 1 1 The effect of an electric ﬁeld can be modelled by including the following term in À xHag Qgb þ dgb À x Qag þ dag Hgb 3 3 the bulk free-energy density: 1 @f Ea þ 2x Qab þ dab QgnHgn À @aQgn À EaQabEb; ð5Þ 3 @@ Q 12p b gn þ QagHgb À HagQgb: where Ea are the components of the electric ﬁeld, and Ea (here assumed positive) is the dielectric anisotropy of the liquid crystal. The strength of the electric ﬁeld is A lattice Boltzmann ﬂow solver is used, where the isotropic pressure p0 and viscous quantiﬁed via one further dimensionless number terms are managed directly by the solver (as in a simple Newtonian ﬂuid, of viscosity Z), whereas the divergence of the remaining terms is treated as a local 2 27Ea E ¼ EaEa: ð6Þ force density on the ﬂuid. In all simulations reported the mean ﬂuid density r ¼ 1 32pA g 0 and the viscosity Z ¼ 0.01 (simulations in conﬁned geometry also used enhanced The quantity E is known as the reduced ﬁeld strength. bulk viscosity z ¼ 10Z to ensure numerical stability).
6 NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications & 2014 Macmillan Publishers Limited. All rights reserved. NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954 ARTICLE
Surface boundary conditions for particles. Hydrodynamic boundary conditions 17. Ravnik, M., Alexander, G. P., Yeomans, J. M. & Zumer, S. Three-dimensional for solid objects are handled via the lattice Boltzmann solver. In particular, the colloidal crystals in liquid crystalline blue phases. Proc. Natl Acad. Sci. USA standard method of bounce-back on links is used for both particles and conﬁning 108, 5188–5192 (2011). 43,44 walls . Boundary conditions for the order parameter are set out in ref. 45. 18. Lavrentovich, O. D. Liquid crystals, photonic crystals, metamaterials and In all the simulations reported here the preferred orientation of the director transformation optics. Proc. Natl Acad. Sci. USA 108, 5143–5144 (2011). ﬁeld at the particle surface is normal to the surface. The required nematic director 0 19. Tiribocchi, A., Gonnella, G., Marenduzzo, D., Orlandini, E. & Salvadore, F. at the particle surface in a given location n^a may then be determined from 0 Bistable defect structures In blue phase devices. Phys. Rev. Lett. 107, 237803 geometry alone, and a preferred order parameter Qab is computed via (2011). 20. Fukuda, J.-I. & Zumer, S. Quasi-two-dimensional Skyrmion lattices in a chiral 0 0 0 0 1 Qab¼q n^an^b À dab : ð15Þ nematic liquid crystal. Nat. Commun. 2, 246 (2011). 3 21. Henrich, O., Marenduzzo, D., Stratford, K. & Cates, M. E. Thermodynamics of blue phases in electric ﬁelds. Phys. Rev. E 81, 031706 (2010). The magnitude of surface order q0 is set by 22. Heikenfeld, J., Drzaic, P., Yeo, J. S. & Koch, T. A critical review of the present 2 1 3 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ and future prospects for electronic paper. J. Soc. Inf. Display 19, 129–156 q0¼ þ 1 þð8=3gÞ ð16Þ (2011). 3 4 4 23. Henrich, O., Stratford, K., Marenduzzo, D. & Cates, M. E. Ordering dynamics that corresponds to the bulk order in a defect-free nematically ordered sample46 of blue phases entails kinetic stabilization of amorphous networks. Proc. Natl (this is also very close to the value of the order parameter in a cholesteric or in a BP Acad. Sci. USA 107, 13212–13215 (2010). away from disclinations). 24. Lintuvuori, J. S., Stratford, K., Cates, M. E. & Marenduzzo, D. Colloids in In all simulations, the colloidal (hard sphere) radius is R ¼ 2.3. To prevent cholesterics: size-dependent defects and non-Stokesian microrheology. Phys. particles overlapping at the hard sphere radius, an additional short range soft Rev. Lett. 105, 178302 (2010). potential is included. This takes the form of VhðÞ¼Eðs=hÞ where h is the surface to 25. Lintuvuori, J. S., Stratford, K., Cates, M. E. & Marenduzzo, D. Self-assembly and surface separation. The parameters are E¼0:0004 and s ¼ 0.1 in simulation units. nonlinear dynamics of dimeric colloidal rotors in cholesterics. Phys. Rev. Lett. Both potential and resulting force are smoothly matched to zero at a cutoff distance 107, 267802 (2011). of hc ¼ 0.25 simulation units. 26. Ravnik, M., Fukuda, J.-I., Yeomans, J. M. & Zumer, S. Conﬁning blue phase colloids to thin layers. Soft Matter 7, 10144–10150 (2011). 27. Helfrich, W. Capillary ﬂow of cholesteric and smectic liquid crystals. Phys. Rev. Surface boundary conditions for walls The conﬁning solid walls, which are ﬂat . Lett. 23, 372–374 (1969). and stationary, have the same normal boundary condition as at the particle surface. 28. Dupuis, A., Marenduzzo, D., Orlandini, E. & Yeomans, J. M. Rheology of In addition, degenerate planar anchoring is applied at the walls, where the pre- cholesteric blue phases. Phys. Rev. Lett. 95, 097801 (2005). ferred nematic director may adopt any orientation parallel to the surface. The 29. Zapotocky, M., Ramos, L., Poulin, P., Lubensky, T. C. & Weitz, D. A. preferred direction is determined explicitly by projecting the local ﬂuid order parameter to the plane of the wall41. Equation (15) and equation (16) are then used Particle-stabilized defect gel in cholesteric liquid crystals. Science 283, 209–212 as before. (1999). To prevent the particles being forced into the wall, a correction to the 30. Ramos, L., Zapotocky, M., Lubensky, T. C. & Weitz, D. A. Rheology of lubrication force on the colloidal particle is added for very low particle surface to defect networks in cholesteric liquid crystals. Phys. Rev. E 66, 031711 wall surface separations ho0.5 lattice spacing. The correction is based on the (2002). analytic expression for the lubrication between a sphere and a ﬂat surface. 31. Hijnen, N., Wood, T. A., Wilson, D. & Clegg, P. S. Self-organization of particles with planar surface anchoring in a cholesteric liquid crystal. Langmuir 26, 13502–13510 (2010). References 32. Yoshida, H. et al. Nanoparticle-stabilized cholesteric blue phases. Appl. Phys. 1. Ravnik, M. et al. Entangled nematic colloidal dimers and wires. Phys. Rev. Lett. Express 2, 121501 (2009). 99, 247801 (2007). 33. Karatairi, E. et al. Nanoparticle-induced widening of the temperature range of 2. Musevic, I., Skarabot, M., Tkalec, U., Ravnik, M. & Zumer, S. Two-dimensional liquid-crystalline blue phases. Phys. Rev. E 81, 041703 (2010). nematic colloidal crystals self-assembled by topological defects. Science 313, 34. Dierking, I. et al. Stabilising liquid crystalline blue phases. Soft Matter 8, 954–958 (2006). 4355–4362 (2012). 3. Araki, T. & Tanaka, H. Colloidal aggregation in a nematic liquid crystal: 35. Draper, M. et al. Self-assembly and shape morphology of liquid crystalline gold topological arrest of particles by a single-stroke disclination line. Phys. Rev. Lett. metamaterials. Adv. Func. Mater. 21, 1260–1278 (2011). 97, 127801 (2006). 36. Milette, J. et al. Reversible long-range network formation in gold nanoparticle- 4. Wood, T. A., Lintuvuori, J. S., Schoﬁeld, A. B., Marenduzzo, D. & nematic liquid crystal composites. Soft Matter 8, 173–179 (2012). Poon, W. C. K. A self-quenched defect glass in a colloid-nematic liquid crystal 37. Cordoyiannis, G. et al. Different modulated structures of topological composite. Science 333, 79–83 (2011). defects stabilized by adaptive targeting nanoparticles. Soft Matter 9, 3956–3964 5. Stark, H. Physics of colloidal dispersions in nematic liquid crystals. Phys. Rep. (2013). 351, 387–474 (2001). 38. Henrich, O., Stratford, K., Coveney, P. V., Cates, M. E. & Marenduzzo, D. 6. Lin, I. H. et al. Endotoxin-induced structural transformations in liquid Rheology of cubic blue phases. Soft Matter 9, 10243–10256 (2013). crystalline droplet. Science 332, 1297–1300 (2011). 39. Psaltis, D., Quake, S. R. & Yang, C. Developing optoﬂuidic technology through 7. Chari, K., Rankin, C. M., Johnson, D. M., Blanton, T. N. & Capurso, R. G. the fusion of microﬂuidics and optics. Nature 442, 381–386 (2006). Single-substrate cholesteric liquid crystal displays by colloidal self-assembly. 40. de Gennes, P.-G. & Prost, J. The Physics of Liquid Crystals (Clarendon Press, Appl. Phys. Lett. 88, 043502 (2006). 1995). 8. Araki, T., Buscaglia, M., Bellini, T. & Tanaka, H. Memory and topological 41. Fournier, J.-B. & Galatola, P. Modeling planar degenerate wetting and frustration in nematic liquid crystals conﬁned in porous materials. Nat. Mater. anchoring in nematic liquid crystals. Europhys. Lett. 72, 403–409 (2005). 10, 303–309 (2011). 42. Beris, A. N. & Edwards, B. J. Thermodynamics of Flowing Systems with Internal 9. Wright, D. C. & Mermin, N. D. Crystalline liquids: the blue phases. Rev. Mod. Microstructure (Oxford University Press, 1994). Phys. 61, 385–432 (1989). 43. Ladd, A. J. C. Numerical simulation of particulate suspensions via a discretized 10. Henrich, O., Stratford, K., Cates, M. E. & Marenduzzo, D. Structure of blue Boltzmann equation. Part 1. Theoretical foundation. J. Fluid Mech. 271, phase III of cholesteric liquid crystals. Phys. Rev. Lett. 106, 107802 (2011). 285–309 (1994). 11. Kikuchi, H., Yokota, M., Hisakado, Y., Yang, H. & Kajiyama, T. Polymer- 44. Nguyen, N.-Q. & Ladd, A. J. C. Lubrication corrections for lattice Boltzmann stabilized liquid crystal blue phases. Nat. Mater. 1, 64–68 (2002). simulations of particle suspensions. Phys. Rev. E 66, 046708 (2002). 12. Cao, W. Y., Munoz, A., Palffy-Muhoray, P. & Taheri, B. Lasing in a three- 45. Lintuvuori, J. S., Marenduzzo, D., Stratford, K. & Cates, M. E. Colloids in dimensional photonic crystal of the liquid crystal blue phase II. Nat. Mater. 1, liquid crystals: a lattice Boltzmann study. J. Mater. Chem. 20, 10547–10552 111–113 (2002). (2010). 13. Coles, H. J. & Pivnenko, M. N. Liquid crystal ‘blue phases’ with a wide 46. Denniston, C., Orlandini, E. & Yeomans, J. M. Lattice Boltzmann simulations temperature range. Nature 436, 997–1000 (2005). of liquid crystal hydrodynamics. Phys. Rev. E 63, 056702 (2001). 14. Ge, Z. B., Gauza, S., Jiao, M. Z., Xianyu, H. Q. & Wu, S. T. Electro-optics of polymer-stabilized blue phase liquid crystal displays. Appl. Phys. Lett. 94, 101104 (2009). 15. Castles, F. et al. Blue-phase templated fabrication of three-dimensional Acknowledgements nanostructures for photonic applications. Nat. Mater. 11, 599–603 (2012). We acknowledge support by UK EPSRC grants EP/J007404/1 (K.S. and J.S.L.), EP/ 16. Ravnik, M., Alexander, G. P., Yeomans, J. M. & Zumer, S. Mesoscopic G036136/1 (O.H.), and EP/I030298/1 (K.S. and J.S.L.). M.E.C. is supported by the Royal modelling of colloids in chiral nematics. Faraday Discuss. 144, 159–169 (2010). Society. We thank both Hector and PRACE for computational resources.
NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications 7 & 2014 Macmillan Publishers Limited. All rights reserved. ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/ncomms4954
Author contributions Competing ﬁnancial interests: The authors declare no competing ﬁnancial interests. K.S., O.H. and J.S.L. contributed to the code base for simulation and performed simu- Reprints and permission information is available online at http://npg.nature.com/ lations. All authors helped to analyse the results and write the manuscript. reprintsandpermissions/ Additional information How to cite this article: Stratford, K. et al. Self-assembly of colloid-cholesteric Supplementary Information accompanies this paper at http://www.nature.com/ composites provides a possible route to switchable optical materials. Nat. Commun. 5:3954 doi: 10.1038/ncomms4954 (2014). naturecommunications
8 NATURE COMMUNICATIONS | 5:3954 | DOI: 10.1038/ncomms4954 | www.nature.com/naturecommunications & 2014 Macmillan Publishers Limited. All rights reserved.